81 pág.

## Pré-visualização | Página 2 de 12

nm Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-10 3.9 This problem asks for us to calculate the radius of a tantalum atom. For BCC, n = 2 atoms/unit cell, and VC = 4 R 3 ⎛ ⎝ ⎜ ⎞ ⎠ ⎟ 3 = 64 R 3 3 3 Since, from Equation 3.5 ρ = nATa VC N A = nATa 64 R3 3 3 ⎛ ⎝ ⎜ ⎜ ⎞ ⎠ ⎟ ⎟ N A and solving for R the previous equation R = 3 3nATa 64ρ N A ⎛ ⎝ ⎜ ⎜ ⎞ ⎠ ⎟ ⎟ 1/3 = (3 3) (2 atoms/unit cell) (180.9 g/mol) (64)(16.6 g/cm3)(6.023 x 1023 atoms/mol) ⎡ ⎣ ⎢ ⎢ ⎤ ⎦ ⎥ ⎥ 1/3 = 1.43 x 10-8 cm = 0.143 nm Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-11 3.10 For the simple cubic crystal structure, the value of n in Equation 3.5 is unity since there is only a single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R (Figure 3.23). Therefore, employment of Equation 3.5 yields ρ = nA VC N A = nA (2 R)3 N A = (1 atom/unit cell)(74.5 g/mol) (2)(1.45 x 10-8 cm) ⎡ ⎣ ⎢ ⎤ ⎦ ⎥ 3 /(unit cell) ⎧ ⎨ ⎪ ⎩ ⎪ ⎫ ⎬ ⎪ ⎭ ⎪ (6.023 x 1023 atoms/mol) 5.07 g/cm3 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-12 3.11 (a) The volume of the Ti unit cell may be computed using Equation 3.5 as VC = nATi ρN A Now, for HCP, n = 6 atoms/unit cell, and for Ti, ATi = 47.9 g/mol. Thus, VC = (6 atoms/unit cell)(47.9 g/mol) (4.51 g/cm3)(6.023 x 1023 atoms/mol) = 1.058 x 10-22 cm3/unit cell = 1.058 x 10-28 m3/unit cell (b) From part of the solution to Problem 3.6, for HCP VC = 6 R 2c 3 But, since a = 2R, (i.e., R = a/2) then VC = 6 a 2 ⎛ ⎝ ⎜ ⎞ ⎠ ⎟ 2 c 3 = 3 3 a2c 2 but, since c = 1.58a VC = 3 3 (1.58) a3 2 = 1.058 x 10-22 cm3/unit cell Now, solving for a a = (2)(1.058 x 10 -22 cm3) (3)( 3) (1.58) ⎡ ⎣ ⎢ ⎢ ⎤ ⎦ ⎥ ⎥ 1/3 = 2.96 x 10-8 cm = 0.296 nm And finally c = 1.58a = (1.58)(0.296 nm) = 0.468 nm Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-13 3.12 This problem asks that we calculate the theoretical densities of Al, Ni, Mg, and W. Since Al has an FCC crystal structure, n = 4, and VC = 16R 3 2 (Equation 3.4). Also, R = 0.143 nm (1.43 x 10-8 cm) and AAl = 26.98 g/mol. Employment of Equation 3.5 yields ρ = nAAl VC N A = (4 atoms/unit cell)(26.98 g/mol) (2)(1.43 x 10-8 cm)( 2)[ ]3/(unit cell)⎧ ⎨ ⎩ ⎫ ⎬ ⎭ (6.023 x 1023 atoms/mol) = 2.71 g/cm3 The value given in the table inside the front cover is 2.71 g/cm3. Nickel also has an FCC crystal structure and therefore ρ = (4 atoms/unit cell)(58.69 g/mol) (2)(1.25 x 10-8 cm)( 2)[ ]3/(unit cell )⎧ ⎨ ⎩ ⎫ ⎬ ⎭ (6.023 x 1023 atoms/mol) = 8.82 g/cm3 The value given in the table is 8.90 g/cm3. Magnesium has an HCP crystal structure, and from the solution to Problem 3.6, VC = 3 3 a2c 2 and, since c = 1.624a and a = 2R = 2(1.60 x 10-8 cm) = 3.20 x 10-8 cm VC = (3 3)(1.624)(3.20 x 10-8 cm)3 2 = 1.38 x 10−22 cm3/unit cell Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is ρ = nAMg VC N A Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-14 = (6 atoms/unit cell)(24.31 g/mol) (1.38 x 10-22 cm3/unit cell)(6.023 x 1023 atoms/mol) = 1.75 g/cm3 The value given in the table is 1.74 g/cm3. Tungsten has a BCC crystal structure for which n = 2 and a = 4 R 3 (Equation 3.3); also AW = 183.85 g/mol and R = 0.137 nm. Therefore, employment of Equation 3.5 leads to ρ = (2 atoms/unit cell)(183.85 g/mol) (4)(1.37 x 10-8 cm) 3 ⎡ ⎣ ⎢ ⎢ ⎤ ⎦ ⎥ ⎥ 3 /(unit cell) ⎧ ⎨ ⎪ ⎩ ⎪ ⎫ ⎬ ⎪ ⎭ ⎪ (6.023 x 1023 atoms/mol) = 19.3 g/cm3 The value given in the table is 19.3 g/cm3. Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-15 3.13 In order to determine whether Nb has an FCC or a BCC crystal structure, we need to compute its density for each of the crystal structures. For FCC, n = 4, and a = 2 R 2 (Equation 3.1). Also, from Figure 2.6, its atomic weight is 92.91 g/mol. Thus, for FCC (employing Equation 3.5) ρ = nANb a3N A = nANb (2R 2)3N A = (4 atoms/unit cell)(92.91 g/mol) (2)(1.43 × 10-8 cm)( 2)[ ]3 /(unit cell)⎧ ⎨ ⎩ ⎫ ⎬ ⎭ (6.023 × 1023 atoms /mol) = 9.33 g/cm3 For BCC, n = 2, and a = 4 R 3 (Equation 3.3), thus ρ = nANb 4 R 3 ⎛ ⎝ ⎜ ⎜ ⎞ ⎠ ⎟ ⎟ 3 N A ρ = (2 atoms/unit cell)(92.91 g/mol) (4)(1.43 × 10-8 cm) 3 ⎡ ⎣ ⎢ ⎢ ⎤ ⎦ ⎥ ⎥ 3 /(unit cell) ⎧ ⎨ ⎪ ⎩ ⎪ ⎫ ⎬ ⎪ ⎭ ⎪ (6.023 × 1023 atoms /mol) = 8.57 g/cm3 which is the value provided in the problem statement. Therefore, Nb has a BCC crystal structure. Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3-17 ρ = nAC 4R 3 ⎛ ⎝ ⎜ ⎞ ⎠ ⎟ 3 N A = (2 atoms/unit cell)(91.6 g/mol) (4)(1.37 × 10-8 cm) 3 ⎡ ⎣ ⎢ ⎢ ⎤ ⎦ ⎥ ⎥ 3 /(unit cell) ⎧ ⎨ ⎪ ⎩ ⎪ ⎫ ⎬ ⎪ ⎭ ⎪ (6.023 × 1023 atoms/mol) = 9.60 g/cm3 Therefore, its crystal structure is BCC. Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled